Complex Permittivity and Permeability Studies Viewing Antenna Applications of NBR-Based Composites Comprising Conductive Fillers

The work presents studies on the complex permittivity and permeability of composites based on acrylonitrile butadiene rubber containing combinations of conductive fillers which include carbon black and nickel powder. The properties of those composites, containing each of the fillers at the same amount were compared. The permittivity and permeability values of the composites are influenced remarkably by their morphology and structure as well as by the morphological and structural specifics of both fillers. As electron scanning microscopy studies confirm, those parameters are predetermined by the nature of the composites studied—particle size, particles arrangement in the matrix and their tendency to clustering. Last but not least matrix-filler interface phenomena also impact the characteristics in question. The possibilities for applications of the composites in antennae have been studied, in particular, as substrates and insulating layers in flexible antennae for body centric communications (BCCs). The research results allow the conclusion that these materials can find such applications indeed. Composites of higher conductivity can be used where surface waves are generated to provide on-body communications, while composites of lower conductivity may be used for antennae that will be on the body of a person and will transmit to and receive from other antennas that are not on the body of the same person (off-body communications). It is clear that one can engineer the properties of How to cite this paper: Al-Sehemi, A.G., Al-Ghamdi, A.A., Dishovsky, N.T., Atanasov, N.T. and Atanasova, G.L. (2018) Complex Permittivity and Permeability Studies Viewing Antenna Applications of NBR-Based Composites Comprising Conductive Fillers. Materials Sciences and Applications, 9, 883-899. https://doi.org/10.4236/msa.2018.911064 Received: September 10, 2018 Accepted: October 23, 2018 Published: October 26, 2018 Copyright © 2018 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY 4.0). http://creativecommons.org/licenses/by/4.0/


Introduction
The current expansion of high-frequency wireless devices and appliances has augmented the need of versatile dielectric antennae, hence urged the search of materials able to meet the producers' requirements-higher dielectric constant and lower tangent of dielectric loss angle values being amongst the most important.In the former case a wave will be transmitted faster in the dielectric material [1], while the latter factor leads to suppressed heat generation-induced energy and to a better performance, respectively.Being hard and brittle conventional antenna materials, lack flexibility and are vulnerable to impact [1], so recently elastomer composites have emerged as promising substitutes of traditional ceramics used to make antenna substrates.A rubber substrate antenna has a number of advantages [1] [2]: • One can choose the relative dielectric constant (4 -20) established arbitrarily to be in the 2.2 -12.0 range for flexible substrates [3] At lower dielectric constant values the surface wave losses are related to guided wave broadcast within substrate.Thus the impedance bandwidth of the antenna raises with adequate competence and high gain [4].
• Low tangent dielectric loss angle values (0.01 or lower) As a dissipation factor the tangent of dielectric loss angle (tanδ) describes the amount of power turned into heat in the substrate material.It is defined as the ratio between the imaginary part and real part of the relative permittivity.Its high values result in additional losses in the dielectric substrate, subsequently into higher losses, in reduced radiation efficiency [5].

• Thickness of the dielectric substrate
The dielectric constant and its width determine the bandwidth and competence of a rubber based flexible antenna.A substrate is normally in the range of 0.003λ ≤ h ≤ 0.005λ, whereas λ represents its wavelength.The bandwidth of the flexible antenna at a fixed comparative permittivity may be maximized by selecting an appropriate substrate.We have assumed that, besides by the layers of the elastomer matrix, the electroconductive aggregates and agglomerates could be insulated by introduction of a second less conductive phase to fill the space between the aggregates and agglomerates.The second phase would have its own contribution to the formation of the dielectric and magnetic losses of the composite.For the purpose we have chosen two conductive phases differing completely in their chemical, crystallochemical and crystallographic properties, namely conductive carbon black (CCB) and nickel powder.
The properties of dual systems (rubber-metallic powder) are well-studied but there are few papers dealing with properties of the tertiary ones (rubber-carbon black-metallic powder) and the comparison of the two types of systems comprising the same amount of filler.Such a type of research also deserves interest in view of the large differences in the chemical and structural properties of the fillers used.Also the influence of the components ratio on the microwave properties of the composite material and the possibilities for its antenna applications requires special attention.
The present study reports on investigations on the complex permittivity and permeability of acrylonitrile-butadiene based composites containing a combination of conductive fillers including carbon black and nickel powder.It also presents and discusses the comparison between the properties of the dual and tertiary composites containing each of the fillers at the same loading degree, as well as assessment of the possibilities for antenna applications of the developed composites.
Nickel powder with apparent density 1.8 -2.7 g/cm 3 and average particles size 3 -7 microns, produced by Alfa Aesar was also used as filler.

Sample Preparation
The formulation of the NBR based compounds (in phr) were as follows: acrylonitrile butadiene rubber (NBR)-100, zinc oxide-

Experimental Techniques
The electromagnetic parameters (EM) of the composite materials were measured by the resonant perturbation method described in a previous publication [6].
According to the resonant perturbation method, the tested sample was introduced into a cavity resonator with dimensions 61.2 mm × 10.0 mm × 610 mm.The EM parameters of the sample were deduced from the change in the resonant frequency and quality factor of the resonator [6].For permittivity measurements the sample was placed at the spot of maximum intensity of electric field, where TE 103 mode was always adopted.For permeability measurements the sample was placed at the spot of maximum magnetic field, where TE 104 even mode was always adopted.

Scanning electron microscopy (SEM)
The nickel powder, CCB and NBR-based composites were subjected to electron microscopy studies on a JEOL ISM 5510 microscope.The SEM images of the nickel powder sample were taken directly and those of carbon black-from aqueous dispersion.The prepared samples were put into a JEOL JFC-1200 cathode-sputtering chamber and covered with 24 carat gold.

Results and Discussion
Figure 1 and Figure 2 present the real ( r ε ′ ) and imaginary ( r ε ′′ ) part of the rela- tive dielectric permittivity of NBR-based vulcanizates at a different filler concentration and 2.56 GHz.As seen, the values for all vulcanizates increase with increasing the filler concentration.The smallest variation is observed for the composites containing only nickel powder, while the highest r ε ′ and r ε ′′ values are observed for composite NBR-6 containing CCB at 60 phr.The results also show that at filler concentration of 30 phr and 50 phr r ε ′ and r ε ′′ values are higher for the tertiary systems, if compared to those of the composites containing only CCB or nickel powder.The opposite is observed at a 60 phr filler loading-the composites with only conductive carbon black have better results.That might be due to the combination of fillers, namely to their different particles shape and Table 1.Formulations of the studied NBR based compounds (in phr).size which yield non-uniform interface phenomena.Hotta et al. [7] discussing the complex permittivity, claim it to be dependent on the specific surface area of the fillers.In our case CCB has specific surface area much higher than that of the nickel powder.The difference in particle size is also huge.
The magnitude of the dielectric loss angle is greatest with NBR-6 composite containing 60 phr carbon black as a filler, whereas at the concentration of 30 phr and 50 phr the values of r ε ′ and r ε ′′ are higher in the triple systems, relative to those composites which contain as filler only carbon black or only nickel powder (Figure 3).These results are due to the fact that the dielectric losses in a multiple composite are the result of complex phenomena like natural resonance, dipole relaxation, electronic polarization as well as their relaxation and interfacial polarizations.Interfacial polarizations occur in heterogeneous media due to accumulation of charges at the interfaces and the formation of large dipoles [8].
The important factor is also the ratio between the particles of the fillers and the host materials [9].The morphology and structure of the conductive filler, its size and shape, as well as the morphology and structure of the composite affect the changes in the real and imaginary part of the relative permittivity.Materials Sciences and Applications The electric conductivity (σ АС ) of the composites at 2.66 GHz is presented in  The results reveal that the increasing filler concentration leads to significant changes in r µ′ and r µ′′ for NBR-1, NBR-2, NBR-3 comprising a hybrid filler and for those with carbon black (NBR-4, NBR-5, NBR-6), while for those loaded with nickel powder the change is negligible.The magnetic losses for magnetic materials originate mainly from domain resonance, hysteresis loss, eddy current loss, and natural resonance.The domain wall resonance normally occurs at a frequency lower than 100 MHz, so it can be neglected in the microwave range.Having measured relative permeability a low microwave power (≤5 mW), we claim that complex phenomena like eddy current loss and natural resonance are the main cause of the magnetic loss in the present study [10], instead of hysteresis and domain resonance observed in the conventional case.Undoubtedly, the morphology and structure of the composites studied influence the mentioned phenomena.
The explanations made are supported by the results obtained by scanning electron microscopy.Figure 8 shows different crystalline structures and formations of layered structure in the investigated nickel powder.
The aggregates of the nickel particles form crystalline structures of the "spiral rosette" type.The rosettes aggregate according to the forces of interaction between them and strive to have a pseudospheric shape.Spheres can also form tiles that make up twin-nano domains.The spiral growth of nano-twins forms the crystal "comb" structure (Figure 8(b)).
Figure 9 shows a SEM image of the used conductive carbon black Printex XE-2B.The picture shows the high structurality of the carbon black expressed via formation of chain aggregates, as well as the tendency of the latter to form agglomerates.Elementary particles are nano-sized.
Figure 10 shows SEM images of the investigated vulcanizates filled at 30 phr.
It is clear from Figure 10  Here in some places we can see the aggregates and agglomerates of the nickel particles, which stand out in their larger dimensions, but the chain-like structures of CCB particles, which act as conducting paths, predominate in the elastomeric matrix.The similarity in the morphology of the two composites also explains their close values of specific volume resistivity, electrical conductivity, respectively.The images obtained by SEM demonstrate clearly that the particles and aggregates are well dispersed in the elastomeric matrix in all composites filled with CCB unlike the nickel powder particles.However, in the presence of carbon black, the dispersion of nickel particles is better.The presented results from SEM studies on the composites confirm categorically that the differences observed in the values of their dielectric permittivity and magnetic permeability, and the tangents of the dielectric and magnetic losses angles are due to significant differences in morphology and structure of the very fillers and of composites filled with the latter.Obviously, the morphology and structure have a significant impact on the phenomena forming the dielectric permittivity and magnetic permeability values described above.It is also obvious that, the morphology and structure of the fillers used are very different.As seen, the particle size and occurrence of particles clustering, the arrangement of the particles in the matrix and the phenomena in the interface region between the matrix and the filler have a significant effect on the permittivity and permeability of the composite materials investigated.
The different types of vulcanizates studied were built into a microwave dipole antenna with a reflector as substrates or insulating layers in flexible antenna for body centric communications (BCCs).The constructed model antenna had three metallic (Figure 12(a)-layers 1, 3 and 5) and three polymer layers (Figure 12(a), layers 2, 4 and 6), and can operate in the industrial, scientific, and medical (ISM) band in the range of 2.40 -2.48 GHz.Materials Sciences and Applications (formulations in Table 1) were used in layer 6.The structure of the antenna as well as its dimensions are shown in Figure 12.The electromagnetic parameters of the NRK composite measured at 2.56 GHz are as follows: r ε ′ = 2.48, r ε ′′ = 0.02, tanδ ε = 0.006, σ АС = 0.0021.
The first series of studies we conducted aimed at showing the absorption of electromagnetic energy from each composite with a conductive filler, while the subsequent studies aim at demonstrating the applicability of the composites to reduce the specific absorption rate (SAR) which is a value that measures how much power is absorbed in a biological tissue when the body is exposed to electromagnetic radiation [11].SAR is determined as follows: where E is the electric field (V/m), σ is the conductivity (S/m), and ρ is the density (kg/m 3 ) [12].
The SAR was computed using FDTD numerical technique by placing a homogeneous human body model (Figure 12(c)) near the antenna.In the course of the study, numerical models of nine antennae were constructed, in each of which the last antenna layer (Layer 6 located behind the reflector) consisted of Materials Sciences and Applications one of the composites from NBR-1 to NBR-9.Table 2 presents the materials from which the individual layers of the investigated antennae were made.Each antenna is placed directly on the surface of the flat phantom composites from NBR-1 to NBR-9.Each antenna is placed directly on the surface of the flat phantom to study how the insulating layer consisting of one of the composites with conductive fillers (NBR-1 to NBR-9) reduces SAR. Figure 13 shows results for the maximum mean 10 g average SAR in each of the composites with conductive fillers (NBR-1 to NBR-9  (FDTD).All results were normalized to a net input power level of 100 mW.As seen, the lowest electromagnetic was power absorbed by the sixth layer of the antenna when it is made of composite NBR-7.This effect can be related to several factors, namely to the lower dielectric permittivity of the composite, lower dielectric losses, and lower conductivity regarding the composites with a conductive filler.Figure 14 shows results for the distribution of SAR over the flat phantom surface caused by an antenna whose last layer is made of one of the composites with the conductive filler (NBR-1 to NBR-9).
According to the above figure, the highest SAR values of the surface of the phantom are observed when the last layer of the antenna is made of composites NBR-2, NBR-3 and NBR-6.These results can be related to the conductivity of the three composites which are higher than that of the rest (Figure 4).High conductivity leads to a current flow both on the surface of the reflector and on the surface of the last composite layer, which in turn leads to the generation of surface waves on the surface of the flat phantom and hence to higher SAR values.It should be noted that, the highest SAR value induced at an input power of 100 mW is lower than the maximum one set in international standards and recommendations [13] [14].On the other hand, the generation of surface waves can be used when the two antennas (transmitting and receiving) are located on the surface of the human body, for example in cases of on-body communications in Body area networks.Analyzing the results in Figure 14, one also sees that antennae with NBR-7, NBR-8 and NBR-9 composites in the third layer of the antenna cause the lowest SAR values of the flat phantom surface.This result may be associated with several factors, namely, the lower dielectric permittivity of the As a result of the research we can conclude that the studied composites can find application as insulating layers and substrates in flexible antennas, depending on the antenna application.For example, composites of higher conductivity can be used in applications where surface waves are generated to realize on-body communications, whereas composites with lower conductivity can be used for antennas that will be on the body of a person and will transmit to and receive from other antennas that are not on the same person's body (off-body communications).It is clear that we can engineer the properties of an antenna substrate at microwave frequencies by adjusting the content and type of the filler and thus control the antenna performance.It will allow us to tailor an antenna performance specific to a particular application.

Conclusions
The complex permittivity and permeability of composites containing conductive fillers-very different in their type and chemical nature-conductive carbon black, nickel powder, and combinations thereof-were investigated.The properties of the dual and tertiary composites were evaluated at the same degree of filling.A noticeable influence of the morphology and structure of both fillers and the composites on their permittivity and permeability values was established.It can be argued that particle size and occurrence of particle clustering; arrangement of the particles in the matrix and phenomena in the interface region between the matrix and the filler are the crucial factors for the permittivity and permeability formation of the composite materials investigated.
The investigations covered the possibilities to use the composites in antennae making, in particular as substrates and insulating properties in body centric communications (BCCs) flexible antennas.The research allows the conclusion that the studied composites can be used for such purposes depending on the application of the antenna.Higher conductivity composites can be used in applications where surface waves are generated to provide on-body communications, while lower conductivity composites may be used for antennas that will be on the body of a person and will transmit to and receive from other antennas that are not on the body of the same person (off-body communications).It is clear that one can engineer the antenna substrate properties at microwave frequencies by adjusting the content and type of filler and thus control and tailor the antenna performances specific to particular applications.

Figure 1 .
Figure 1.Real part of the relative dielectric permittivity of NBR-based vulcanizates.

Figure 2 .
Figure 2. Imaginary part of the relative dielectric permittivity of NBR-based vulcanizates.

Figure 4 .Figure 3 .
Figure 4.As seen, composites NBR-2, NBR-3, NBR-5 and NBR-6 are highly electroconductive and NBR-6, possesses the highest σ АС values.Compositesconductivity is a function of a number of factors, but filler-filler and matrix-filler interactions are the determining ones[6].The higher the filler loading in the matrix, the more the conductive paths in it are.Another factor is the so called "percolation threshold"-a certain concentration of the filler that causes a drastic conductivity increase.The number of conductive paths continues to increase at filler amounts higher than the percolation threshold.That leads to the formation of a complete conducting network, which can explain the high σ АС value for NBR-6, as the percolation threshold for Printex is at about 25 phr.The results in Figure4allow the conclusion that the tertiary systems have σ АС values higher than those of the composites loaded only with one filler at the same amount (30 phr and 50 phr).As Figure4, shows σ АС (NBR-1) > σ АС (NBR-4) > σ АС (NBR-7)

Figure 5 .
Figure 5. Real part of the relative magnetic permeability of NBR-based vulcanizates.

Figure 6 .
Figure 6.Imaginary part of the relative magnetic permeability of NBR-based vulcanizates.

Figure 11 (Figure 11 .
Figure 11(a) shows clearly the nickel aggregates made up of a large number of particles of different size which are isolated from each other with a coating layer cutting the contact between them.In addition, the aggregates themselves are encapsulated by an elastomeric layer and are located in the matrix itself on separate islands remote from one another.That impedes greatly the charge transfer and blocks the high electrical conductivity of the nickel powder.In the composite, filled with CCB at 60 phr (Figure 11(b)), the location of the carbon black particles in the elastomeric matrix is identical to that of the composite filled with

Figure 12 .
Figure 12.Structure of the antenna (a), photograph of the antenna (b) and photograph of the homogeneous flat phantom (c).

Figure 13 .
Figure 13.Maximum averaged 10 g SAR values caused by investigated antennaе in composite layers and flat phantom.

Figure 14 .
Figure 14.SAR distribution over the flat phantom and antenna when Layer 6 is made of composites NBR-1 to NBR-9.

Table 2 .
).The 12-field components approach was used to calculate SAR in the voxel using xFDTD (xFDTD, Remcom Inc., State College, PA, USA) simulation software, based on the finite-difference time domain method Materials used to build the layers of the antennae studies.